WHI Formula as a New Criterion in Automatic Pipeline GMAW Process


 Katherine Johns
 1 years ago
 Views:
Transcription
1 4 WHI Formula as a New Criterion in Automatic Pipeline GMAW Process Alireza Doodman Tipi and Fatemeh Sahraei Kermanshah University of Technology, Pardis, Kermanshah, Iran 1. Introduction Pipeline welding is one of the most significant applications of GMAW process. Automatic welding for pipelines has been developed from early 1970 s. In these systems the welding robot moves around the two pipe's seam and welds the pipes by arc welding machine. Depending on the pipe thickness, weld process is repeated in several passes while the seam is filled of weld mass. The automatic pipeline welding systems has been recently paid more attention [1, 2]. In order to achieve sufficient performance in the process, the input parameters must be chosen correctly [3]. Welding parameter designing is a complicated step in the GMAW process, because of the large number of parameters and complexity of dynamic behavior. This complexity is particularly intensified in automatic pipeline systems, because of the complex seam geometry, wide range of the angle variations and strict quality requirements [1]. The most important input parameters in the automatic pipeline GMAW process are: welding current, arc voltage, travel speed, wire feeding speed, Contact Tube to Workpiece Distance (CTWD), welding position (angle), gas type, pipe type/thickness and seam geometry [4, 5]. The output parameters of the process are usually defined as either mechanical properties or weld bead geometry [6]. Weld bead geometry method considers the relationships between the input parameters and weld bead dimensions (penetration, width, reinforcement height, and width to penetration ratio and dilution [3, 7, 8]. Appropriate melting of the seam walls is certainly one of the most important conditions to achieve a proper dimension in fusion zone. A fusion zone with a sufficient width is necessary to prevent from some defects like lack of Fusion (LOF) [9, 10]. Having a direct contact between the arc and seam walls and receiving enough energy to the walls led to suitable wall melting and appropriate fusion zone [11, 12]. Some criteria such as heat input are related to the total energy which is given to the weld region without considering the amount of energy required to melt the wire. Principal parameters to calculate the heat input value are: welding current, arc voltage, travel speed and welding efficiency [11, 13]. During the welding process, part of the arc energy is spent to melt the wire [12]. Seam geometry also plays an important role in the amount of arc energy that directly reaches the walls. However a more general formula is not yet introduced.
2 72 Arc Welding In this paper WHI introduced as a new criterion, which is related to the arc energy that directly reaches the walls considering the both required energy to melt the wire and seam geometry. This criterion has the capability to be used for designing the welding parameters and for welding analysis applications. Section 2 contains theoretical parts to achieve WHI criterion, which includes wire melting energy (section 2.1), WHI formula (section 2.2), and wall geometry calculations (section 2.3). In section 3 two experimental tests are performed using the fabricated automatic system [15] in order to validate the obtained results from the presented formula. Value (unit) (mm 2 ) 500 (J/kg. o C) 7800 (kg/m 3 ) (J/mm) 7.7 (J/mm 3 ) (J/mm) (J/mm) (J/mm 2 ) (J/kg) Symbols A A osc c st d st E i E st E w E wall E wd F st Nomenclature Molten area for wire (front view) Torch oscillation amplitude Specific heat for steel Steel density Heat input Energy density for steel melting Wire melting energy Wall energy WHI Heat of fusion for steel (V) (A)  (m/s) (m/s) 27 ( o C) 1510 ( o C) (mm 3 /mm) (deg) (deg) Table 1. Variables and material properties. V I η w s T s r l l a l h l v T 0 T mst R V w W a α δ Arc voltage Welding current Arc radiation lost coefficient Wire feed rate Travel speed Wire radius Wall cross length with molten metal and arc (front view) Arc length Seam floor length (front view) Side wall length (front view) Heat of environment Melting point for steel radius of the seam shape Wire volume per travel speed Arc width Wall angle Arc angle
3 WHI Formula as a New Criterion in Automatic Pipeline GMAW Process WHI theory In this section, firstly the required energy for melting the wire is calculated and the wall length of the groove face in contact with the arc is computed as well, remaining arc energy on the seam walls is named WHI. 2.1 Wire melting energy Weld metal area (cross section, in front of view) is a function of wire radius, wire feeding speed and travel speed. The deposition rate (w s /T s ) is usually considered to be fixed for designing of welding parameters. Therefore the molten metal cross section (A) is counted as an assumed parameter in design procedure. 2 ws A r (1) T The amount of heat input over the length unit of travel axis is computed considering the radiation energy [11]. s s VI Ei (2) T 9 The mass of 1mm 3 steel is equal to kg. Therefore melting of 1mm 3 steel (with 300 o K primary temperature) needs approximately 7.7J energy according to eqn. (3) st st st mst 0 10 st st E d c T T d F (3) The volume of the molten wire poured down inside the seam along l t mm of the travel axis is obtained using eqn. (4) V w Al (4) The value of the required Energy for melting the wire poured inside the seam (versus travel axis unit (J/mm)) can be computed as below: E t E V (5) w st w 2.2 WHI formula Arc energy is spent to melt both the filler wire and the walls (eqn. 6). Therefore the remaining energy which directly contacts and melts the walls is named wall energy (E wall ). Ei Ew Ewall (6) Energy density with respect to the seam wall length is computable through dividing the energy of the wall by the seam wall length (l) (front view). Therefore WHI can be defined as the below equation. E wd Ewall (7) l
4 74 Arc Welding So WHI can be shown by welding parameters as below: E wd VI 2 ws 7.7 r Ts Ts (8) l 2.3 Wall geometry The front view of the arc and bevel for the welding of the first pass in a Utype bevel can be seen in fig.1. Fig. 1. A schematic view of the arc, melting wire area and seam walls The arc width (Fig. 1) is calculated using eqn. (10) [14]. Wa 2latan( ) (9) 2 The wall length involving with the arc edges is calculated by eqn. (1013). Wa 2R l vd sin( ) (10) 2 l vd Wa 2R (11) 2sin( ) lr R (12) l 2l vd l r (13) For the other passes (except for the root pass), front view of the arc and seam (for Utype seam) is like Fig. 2. Seam walls length (front view) involving with the arc edges is computable using eqn. (1415).
5 WHI Formula as a New Criterion in Automatic Pipeline GMAW Process 75 Fig. 2. A schematic view for melting area in the second pass l vu Wa lh (14) 2sin( ) l 2l vu l h (15) If there is torch oscillation amplitude (see Fig. 3) the effective arc width can be computable by eqn. (16) [15]. Wa Aosc 2latan( ) (16) 2 Fig. 3. Seam and arc with nozzle oscillation amplitude
6 76 Arc Welding If the effective arc width is too much compared to the melting wire area, some of the wall energy will be lost over the seam without any involving with the molten metal. Furthermore if the center of the oscillation and the seam centerline are not identical (see Fig. 4(left)), the fusion area in the both sides, will not be same. A schematic view and a real test result are shown in Fig. 4. In this figure the center of the oscillation and the seam centerline do not coincide, additionally, the oscillation amplitude is too much, hence Fig. 4(right) has been resulted in the experiment. Fig. 4. Unsymmetrical and extra amplitude of arc width compared to molten wire area, schematic view (left), real test result (right) 3. Experimental results 3.1 Setup The automatic pipeline welding system used in the experiments [15] has been shown in Fig. 5. The welding progresses downward semicircularly from top (0 ) to the bottom (180 ) of the pipe on each side. The solid wire was ER70S6(SG3), having diameter of 1 mm, the shielding gas is the mixture of Argon and CO 2 by 82/18 proportion.
7 WHI Formula as a New Criterion in Automatic Pipeline GMAW Process 77 Fig. 5. Automatic pipe line welding system in the experiments (made by Novin Sazan Co.) The pipe material is API 5L x65 HSLA steel with the thickness of 20.6 mm and the outside diameter of 32 inches. A Utype joint design is used according to fig6. Seam area is about 130mm 2, that is filled with several weld passes. Fig. 6. Joint configuration in the experiments 3.2 Experiments Ex. 1: WHI value has been chosen equal to 32.3 J/mm 2,the other parameters have been computed as the first row in Table 2 (only root pass parameters are shown). These parameters implemented on the system. Longitudinal cross section of the weld metal (front view) is shown in Fig. 7 (left), moreover root pass reinforcement (from inside the pipe) is shown in Fig. 8 (left). Ex. 1 Ex. 2 V(V) I(A) W s (mm/s) T s (mm/s) A(mm 2 ) L E i (J/mm) WHI(J/mm 2 ) Table 2. Welding parameters for two experimental tests
8 78 Arc Welding The molten base metal area is about 66mm 2. This area is highlighted in Fig. 9 (a). this area has been calculated by computer and image processing algorithms using MATLAB. Base metal molten area over to total molten area (summing of base metal and melting wire area) is defined as relative molten area, is about 34% for this example (Ex. 1). Fig. 7. Front view of the weld sections, 32.3J/mm 2 WHI and 393 J/mm heat input according to Ex. 1parameters (left); 35.2J/mm 2 WHI and 337 J/mm heat input with Ex. 2 parameters (right) Fig. 8. Back view of welds from inside the pipe; for Ex.1 (up) and for Ex. 2 (down), Ex. 2 has more penetration than Ex. 1 related to the more WHI
9 WHI Formula as a New Criterion in Automatic Pipeline GMAW Process 79 Ex. 2: WHI value has been selected equal to 35.2 J/mm 2, and Parameters are calculated according to the WHI value. Welding parameters are shown in the second row of the Table 2 (only for root pass). Comparing parameters of Ex. 1 and Ex. 2 indicates an important point: WHI increases but total heat input decreases because of the decreasing of the wire feeding rate (in Ex. 2 than Ex. 1). Cross section and back view (from inside the pipe) is shown in Fig. 7(right) and Fig. 8(right) respectively. Molten base metal area (walls molten area) is estimated to be about 105 mm 2, which is shown in Fig. 9(b). Relative molten area is also estimated to be about 45%. Because of the more WHI (despite decreasing the heat input), fusion zone and penetration has been increased. Fig. 9. Fusion zones of metal base in Ex. 1 (32.3J/mm 2 WHI) (a), and for Ex. 2 (35.2J/mm 2 ) (b) 4. Conclusion In this paper WHI was introduced as a new criterion for designing of the welding parameters and welding analysis. This criterion calculates some of the heat input that is directly given to the walls from the arc. This formula considers the effects of the both required wire melting energy and seam geometry on the input energy. It was shown that WHI has a more correlation with fusion zone area compared to the heat input formula. In the other view the obtained results can be extended to the other welding processes and other applications. However WHI has a good feature in welding parameters designing to achieve some appropriate welding properties like the fusion zone. 5. References [1] Lopes AGT (2006) ArcBased Sensing in Narrow Groove Pipe Welding. Ph.D. Thesis, Sch. Ind. Manuf. Sci., Cranfield U. [2] Blackman SA, Dorling DV (2000) Advanced welding processes for transmission pipelines. In: 3 rd Int. Conf., Pipeline Technol. Proc. [3] Murugan N, Parmar RS (1994) Effects of MIG process parameters on the geometry of the bead in the automatic surfacing of stainless steel, J Mater Process Technol 41:
10 80 Arc Welding [4] Thomsen JS (2004) Advanced control methods for optimization of arc welding, Ph.D. Thesis, Department of Control Engineering, Aalborg University, Denmark, June [5] Connor LP (1991) Welding handbookwelding processes. 8 th edi. American Welding Society [6] Benyounis KY, Olabi AG (2008) Optimization of different welding processes using statistical and numerical approachesa reference guide, Adv Eng Soft 39: [7] Raveendra J, Parmar RS (1987) Mathematical models to predict weld bead geometry for flux cored arc welding. Journal of Metal Constructions 19: [8] Kim IS, Son JS, Kim IG, Kim OS (2003) A study on relationship between process variable and bead penetration for robotic CO2 arc welding. Journal of Materials Processing Technology 136: [9] Mendez PF, Eagar TW (2003) Penetration and Defect Formation in HighCurrent arc welding, Weld J, 82(10)296s306s [10] Okui N, Ketron D, Bordelon F, Hirata Y, Clark G (2007) A Methodology for Prediction of Fusion Zone Shape, weld J, 35s43s [11] Lancaster JF (1986) The physics of welding. Pergamon Pub., 2 nd edi. [12] Lin ML, Eagar TW (1985) Influence of arc pressure on weld pool geometry, Weld J, s169s [13] Lancaster JF (1993) Metallurgy of welding. Chapman & Hall pub., 5 th edi. [14] Guoxiang XU, Chuansong WU (2007) Numerical analysis of weld pool geometry in globulartransfer gas metal arc welding, Front. Mater. Sci. China, 1(1): [15] Doodman AR, Mortazavi SA (2008) A new adaptive method (AFPID) presentation with implementation in the automatic welding robot, IEEE/ASME Int. Conf. Mechat. Emb. Sys. Appl., (MESA08).
11 Arc Welding Edited by Prof. Wladislav Sudnik ISBN Hard cover, 320 pages Publisher InTech Published online 16, December, 2011 Published in print edition December, 2011 Ever since the invention of arc technology in 1870s and its early use for welding lead during the manufacture of leadacid batteries, advances in arc welding throughout the twentieth and twentyfirst centuries have seen this form of processing applied to a range of industries and progress to become one of the most effective techniques in metals and alloys joining. The objective of this book is to introduce relatively established methodologies and techniques which have been studied, developed and applied in industries or researches. Stateoftheart development aimed at improving technologies will be presented covering topics such as weldability, technology, automation, modelling, and measurement. This book also seeks to provide effective solutions to various applications for engineers and researchers who are interested in arc material processing. This book is divided into 4 independent sections corresponding to recent advances in this field. How to reference In order to correctly reference this scholarly work, feel free to copy and paste the following: Alireza Doodman Tipi and Fatemeh Sahraei (2011). WHI Formula as a New Criterion in Automatic Pipeline GMAW Process, Arc Welding, Prof. Wladislav Sudnik (Ed.), ISBN: , InTech, Available from: InTech Europe University Campus STeP Ri Slavka Krautzeka 83/A Rijeka, Croatia Phone: +385 (51) Fax: +385 (51) InTech China Unit 405, Office Block, Hotel Equatorial Shanghai No.65, Yan An Road (West), Shanghai, , China Phone: Fax:
Sensing and Control. A Process Control Primer
Sensing and Control A Process Control Primer Copyright, Notices, and Trademarks Printed in U.S.A. Copyright 2000 by Honeywell Revision 1 July 2000 While this information is presented in good faith and
More informationAN0971 APPLICATION NOTE
APPLICATION NOTE One Technology Way P.O. Box 9106 Norwood, MA 020629106, U.S.A. Tel: 781.329.4700 Fax: 781.461.3113 www.analog.com Recommendations for Control of Radiated Emissions with isopower Devices
More informationGuide on How to Develop a Small Hydropower Plant
ESHA 2004 Guide on How to Develop a Small Hydropower Plant The present document is an updated version developed by the Thematic Network on Small hydropower (TNSHP) of the Layman s Guidebook on how to develop
More informationTHE development of methods for automatic detection
Learning to Detect Objects in Images via a Sparse, PartBased Representation Shivani Agarwal, Aatif Awan and Dan Roth, Member, IEEE Computer Society 1 Abstract We study the problem of detecting objects
More informationMagnetron Theory of Operation
Magnetron Theory of Operation Theory of Operation A magnetron is a high power microwave oscillator in which the potential energy of an electron cloud near the cathode is converted into r.f. energy in a
More informationRESEARCH REPORT 432. Operator rollover protection on small vehicles HSE
HSE Health & Safety Executive Operator rollover protection on small vehicles Prepared by Silsoe Research Institute for the Health and Safety Executive 2006 RESEARCH REPORT 432 HSE Health & Safety Executive
More informationAgilent Time Domain Analysis Using a Network Analyzer
Agilent Time Domain Analysis Using a Network Analyzer Application Note 128712 0.0 0.045 0.6 0.035 Cable S(1,1) 0.4 0.2 Cable S(1,1) 0.025 0.015 0.005 0.0 1.0 1.5 2.0 2.5 3.0 3.5 4.0 Frequency (GHz) 0.005
More informationHALL EFFECT SENSING AND APPLICATION
HALL EFFECT SENSING AND APPLICATION MICRO SWITCH Sensing and Control 7DEOHRI&RQWHQWV Chapter 1 Hall Effect Sensing Introduction... 1 Hall Effect Sensors... 1 Why use the Hall Effect... 2 Using this Manual...
More informationPrinciples of DirectOperated Regulators
Principles of DirectOperated Regulators Introduction Pressure regulators have become very familiar items over the years, and nearly everyone has grown accustomed to seeing them in factories, public buildings,
More informationHelp File Version 1.0.14
Version 1.0.14 By engineering@optimumg.com www.optimumg.com Welcome Thank you for purchasing OptimumT the new benchmark in tire model fitting and analysis. This help file contains information about all
More informationIEEE TRANSACTIONS ON AUDIO, SPEECH, AND LANGUAGE PROCESSING, 2013. ACCEPTED FOR PUBLICATION 1
IEEE TRANSACTIONS ON AUDIO, SPEECH, AND LANGUAGE PROCESSING, 2013. ACCEPTED FOR PUBLICATION 1 ActiveSet Newton Algorithm for Overcomplete NonNegative Representations of Audio Tuomas Virtanen, Member,
More information(1) I. INTRODUCTION (2)
IEEE TRANSACTIONS ON IMAGE PROCESSING, VOL. 19, NO. 12, DECEMBER 2010 3243 Distance Regularized Level Set Evolution and Its Application to Image Segmentation Chunming Li, Chenyang Xu, Senior Member, IEEE,
More informationA Googlelike Model of Road Network Dynamics and its Application to Regulation and Control
A Googlelike Model of Road Network Dynamics and its Application to Regulation and Control Emanuele Crisostomi, Steve Kirkland, Robert Shorten August, 2010 Abstract Inspired by the ability of Markov chains
More informationDOEI Basic Design of Experiments (The Taguchi Approach)
Complimentary Copy: DOEI Basic Design of Experiments (The Taguchi Approach) Target Mean Target Quality Engineering Seminar and Software Bloomfield Hills, MI, USA. www.nutekus.com Page 2 DOEI Basic Design
More informationSteering User Behavior with Badges
Steering User Behavior with Badges Ashton Anderson Daniel Huttenlocher Jon Kleinberg Jure Leskovec Stanford University Cornell University Cornell University Stanford University ashton@cs.stanford.edu {dph,
More informationG. A. REZNICHENKO, A. A. VYRYPAEV DETAIL DESIGN OF AIRFRAME PART
The Ministry of Education and Science of the Russian Federation Samara State Aerospace University (National Research University) G. A. REZNICHENKO, A. A. VYRYPAEV DETAIL DESIGN OF AIRFRAME PART Electronic
More informationAn introduction to quadrupole timeofflight mass spectrometry
JOURNAL OF MASS SPECTROMETRY J. Mass Spectrom. 21; 36: 849 865 SPECIAL FEATURE: TUTORIAL An introduction to quadrupole timeofflight mass spectrometry Igor V. Chernushevich, Alexander V. Loboda and Bruce
More informationOPRE 6201 : 2. Simplex Method
OPRE 6201 : 2. Simplex Method 1 The Graphical Method: An Example Consider the following linear program: Max 4x 1 +3x 2 Subject to: 2x 1 +3x 2 6 (1) 3x 1 +2x 2 3 (2) 2x 2 5 (3) 2x 1 +x 2 4 (4) x 1, x 2
More informationA Separation Control CFD Validation Test Case Part 2. Zero Efflux Oscillatory Blowing
43 rd AIAA Aerospace Sciences Meeting and Exhibit, Reno, NV 25 A Separation Control CFD Validation Test Case Part 2. Zero Efflux Oscillatory Blowing David Greenblatt, * Keith B. Paschal, ChungSheng Yao
More informationChapter 13 TwoPhase Pressure Drops
Chapter 13 TwoPhase Pressure Drops (Revised in 006) Summary: Accurate prediction of twophase pressure drops in directexpansion and flooded evaporators, in tubeside and shellside condensers, and in
More informationTHE PROBLEM OF finding localized energy solutions
600 IEEE TRANSACTIONS ON SIGNAL PROCESSING, VOL. 45, NO. 3, MARCH 1997 Sparse Signal Reconstruction from Limited Data Using FOCUSS: A Reweighted Minimum Norm Algorithm Irina F. Gorodnitsky, Member, IEEE,
More informationDOE FUNDAMENTALS HANDBOOK
DOEHDBK1019/293 JANUARY 1993 DOE FUNDAMENTALS HANDBOOK NUCLEAR PHYSICS AND REACTOR THEORY Volume 2 of 2 U.S. Department of Energy Washington, D.C. 20585 FSC6910 Distribution Statement A. Approved for
More informationPRINTED CIRCUIT BOARD DESIGN
CHAPTER 6 PRINTED CIRCUIT BOARD DESIGN 6.1 INTRODUCTION The designers are key personnel in the development of a new electronic product but they are not the only ones. A successful product depends on an
More informationA handbook prepared under contract for the Commission of the European Communities, DirectorateGeneral for Energy by European Small Hydropower
A handbook prepared under contract for the Commission of the European Communities, DirectorateGeneral for Energy by European Small Hydropower Association (ESHA) The drawing on the cover, published by
More informationReinitialization Free Level Set Evolution via Reaction Diffusion
1 Reinitialization Free Level Set Evolution via Reaction Diffusion Kaihua Zhang, Lei Zhang, Member, IEEE, Huihui Song and David Zhang, Fellow, IEEE Abstract This paper presents a novel reactiondiffusion
More informationFlow Assurance A System Perspective
MEK4450FMC Subsea technologies Flow Assurance A System Perspective By Tine Bauck IrmannJacobsen Contact: TineBauck.IrmannJacobsen@fmcti.com, MobPhone: 9175 9872 The objective of this part is to familiarize
More informationDOE FUNDAMENTALS HANDBOOK MATHEMATICS Volume 2 of 2
DOEHDBK1014/292 JUNE 1992 DOE FUNDAMENTALS HANDBOOK MATHEMATICS Volume 2 of 2 U.S. Department of Energy Washington, D.C. 20585 FSC6910 Distribution Statement A. Approved for public release; distribution
More informationReduction of Wind and Swell Waves by Mangroves
Natural Coastal Protection Series ISSN 20507941 Reduction of Wind and Swell Waves by Mangroves Anna McIvor, Iris Möller, Tom Spencer and Mark Spalding Natural Coastal Protection Series: Report 1 Cambridge
More informationSingleElectron Devices and Their Applications
SingleElectron Devices and Their Applications KONSTANTIN K. LIKHAREV, MEMBER, IEEE Invited Paper The goal of this paper is to review in brief the basic physics of singleelectron devices, as well as their
More informationFDM Part Quality Manufactured with Ultem*9085
FDM Part Quality Manufactured with Ultem*9085 A. Bagsik 1,2, V. Schöppner 1, E. Klemp 2 1 Kunststofftechnik Paderborn (KTP),Universität Paderborn, D33102 Paderborn, Germany 2 Direct Manufacturing Research
More information